# Chapter 1 ELECTROMAGNETICS of METALS

Chapter 1

ELECTROMAGNETICS OF METALS

While the optical properties of metals are discussed in most textbooks on condensed matter physics, for convenience this chapter summarizes the most important facts and phenomena that form the basis for a study of surface plas- mon polaritons. Starting with a cursory review of Maxwell’s equations, we describe the electromagnetic response both of idealized and real metals over a wide frequency range, and introduce the fundamental excitation of the conduc- tion electron sea in bulk metals: volume plasmons. The chapter closes with a discussion of the electromagnetic energy density in dispersive media.

1.1 Maxwell’s Equations and Electromagnetic Wave Propagation The interaction of metals with electromagnetic ﬁelds can be ﬁrmly under- stood in a classical framework based on Maxwell’s equations. Even metallic nanostructures down to sizes on the order of a few nanometres can be described without a need to resort to quantum mechanics, since the high density of free carriers results in minute spacings of the electron energy levels compared to thermal excitations of energy kBT at room temperature. The optics of met- als described in this book thus falls within the realms of the classical theory. However, this does not prevent a rich and often unexpected variety of optical phenomena from occurring, due to the strong dependence of the optical prop- erties on frequency. As is well known from everyday experience, for frequencies up to the vis- ible part of the spectrum metals are highly reﬂective and do not allow elec- tromagnetic waves to propagate through them. Metals are thus traditionally employed as cladding layers for the construction of waveguides and resonators for electromagnetic radiation at microwave and far-infrared frequencies. In this 6 Electromagnetics of Metals low-frequency regime, the perfect or good conductor approximation of inﬁnite or ﬁxed ﬁnite conductivity is valid for most purposes, since only a negligible fraction of the impinging electromagnetic waves penetrates into the metal. At higher frequencies towards the near-infrared and visible part of the spectrum, ﬁeld penetration increases signiﬁcantly, leading to increased dissipation, and prohibiting a simple size scaling of photonic devices that work well at low frequencies to this regime. Finally, at ultraviolet frequencies, metals acquire dielectric character and allow the propagation of electromagnetic waves, albeit with varying degrees of attenuation, depending on the details of the electronic band structure. Alkali metals such as sodium have an almost free-electron-like response and thus exhibit an ultraviolet transparency. For noble metals such as gold or silver on the other hand, transitions between electronic bands lead to strong absorption in this regime. These dispersive properties can be described via a complex dielectric func- tion ε(ω), which provides the basis of all phenomena discussed in this text. The underlying physics behind this strong frequency dependence of the optical response is a change in the phase of the induced currents with respect to the driving ﬁeld for frequencies approaching the reciprocal of the characteristic electron relaxation time τ of the metal, as will be discussed in section 1.2. Before presenting an elementary description of the optical properties of met- als, we recall the basic equations governing the electromagnetic response, the macroscopic Maxwell equations. The advantage of this phenomenological ap- proach is that details of the fundamental interactions between charged parti- cles inside media and electromagnetic ﬁelds need not be taken into account, since the rapidly varying microscopic ﬁelds are averaged over distances much larger than the underlying microstructure. Speciﬁcs about the transition from a microscopic to a macroscopic description of the electromagnetic response of continuous media can be found in most textbooks on electromagnetics such as [Jackson, 1999]. We thus take as a starting point Maxwell’s equations of macroscopic elec- tromagnetism in the following form:

∇·D = ρext (1.1a) ∇·B = 0 (1.1b) ∂B ∇×E =− (1.1c) ∂t ∂D ∇×H = J + . (1.1d) ext ∂t These equations link the four macroscopic ﬁelds D (the dielectric displace- ment), E (the electric ﬁeld), H (the magnetic ﬁeld), and B (the magnetic induc- Maxwell’s Equations and Electromagnetic Wave Propagation 7 tion or magnetic ﬂux density) with the external charge and current densities ρext and Jext. Note that we do not follow the usual procedure of presenting the macroscopic equations via dividing the total charge and current densities ρtot and Jtot into free and bound sets, which is an arbitrary division [Illinskii and Keldysh, 1994] and can (especially in the case of metallic interfaces) confuse the application of the boundary condition for the dielectric displacement. In- stead, we distinguish between external (ρext, Jext) and internal (ρ,J) charge and current densities, so that in total ρtot = ρext + ρ and Jtot = Jext + J.The external set drives the system, while the internal set responds to the external stimuli [Marder, 2000]. The four macroscopic ﬁelds are further linked via the polarization P and magnetization M by

D = ε0E + P (1.2a) 1 H = B − M, (1.2b) μ0 1 2 where ε0 and μ0 are the electric permittivity and magnetic permeability of vacuum, respectively. Since we will in this text only treat nonmagnetic me- dia, we need not consider a magnetic response represented by M, but can limit our description to electric polarization effects. P describes the electric dipole moment per unit volume inside the material, caused by the alignment of micro- scopic dipoles with the electric ﬁeld. It is related to the internal charge density via ∇·P =−ρ. Charge conservation (∇·J =−∂ρ/∂t) further requires that the internal charge and current densities are linked via ∂P J = . (1.3) ∂t The great advantage of this approach is that the macroscopic electric ﬁeld includes all polarization effects: In other words, both the external and the in- duced ﬁelds are absorbed into it. This can be shown via inserting (1.2a) into (1.1a), leading to ρ ∇·E = tot . (1.4) ε0 In the following, we will limit ourselves to linear, isotropic and nonmagnetic media. One can deﬁne the constitutive relations

D = ε0εE (1.5a)

B = μ0μH. (1.5b)

1 −12 ε0 ≈ 8.854 × 10 F/m 2 −6 μ0 ≈ 1.257 × 10 H/m 8 Electromagnetics of Metals

ε is called the dielectric constant or relative permittivity and μ = 1therela- tive permeability of the nonmagnetic medium. The linear relationship (1.5a) between D and E is often also implicitly deﬁned using the dielectric suscepti- bility χ (particularly in quantum mechanical treatments of the optical response [Boyd, 2003]), which describes the linear relationship between P and E via

P = ε0χE. (1.6) Inserting (1.2a) and (1.6) into (1.5a) yields ε = 1 + χ. The last important constitutive linear relationship we need to mention is that between the internal current density J and the electric ﬁeld E, deﬁned via the conductivity σ by J = σ E. (1.7)

We will now show that there is an intimate relationship between ε and σ , and that electromagnetic phenomena with metals can in fact be described using either quantity. Historically, at low frequencies (and in fact in many theoretical considerations) preference is given to the conductivity, while experimentalists usually express observations at optical frequencies in terms of the dielectric constant. However, before embarking on this we have to point out that the statements (1.5a) and (1.7) are only correct for linear media that do not exhibit temporal or spatial dispersion. Since the optical response of metals clearly depends on frequency (possibly also on wave vector), we have to take account of the non-locality in time and space by generalizing the linear relationships to

D(r,t)= ε0 dt dr ε(r − r ,t − t )E(r ,t ) (1.8a) J(r,t)= dtdrσ(r − r,t − t )E(r,t). (1.8b)

ε0ε and σ therefore describe the impulse response of the respective linear re- lationship. Note that we have implicitly assumed that all length scales are signiﬁcantly larger than the lattice spacing of the material, ensuring homo- geneity, i.e. the impulse response functions do not depend on absolute spatial and temporal coordinates, but only their differences. For a local response, the functional form of the impulse response functions is that of a δ-function, and (1.5a) and (1.7) are recovered. Equations (1.8) simplify signiﬁcantly by taking the Fourier transform with respect to dtdrei(K·r−ωt), turning the convolutions into multiplications. We are thus decomposing the ﬁelds into individual plane-wave components of wave vector K and angular frequency ω. This leads to the constitutive rela- Maxwell’s Equations and Electromagnetic Wave Propagation 9 tions in the Fourier domain

D(K,ω)= ε0ε(K,ω)E(K,ω) (1.9a)

J(K,ω)= σ(K,ω)E(K,ω). (1.9b)

Using equations (1.2a), (1.3) and (1.9) and recognizing that in the Fourier do- main ∂/∂t →−iω, we ﬁnally arrive at the fundamental relationship between the relative permittivity (from now on called the dielectric function)andthe conductivity

iσ(K,ω) ε(K,ω)= 1 + . (1.10) ε0ω

In the interaction of light with metals, the general form of the dielectric re- sponse ε(ω, K) can be simpliﬁed to the limit of a spatially local response via ε(K = 0,ω) = ε(ω). The simpliﬁcation is valid as long as the wavelength λ in the material is signiﬁcantly longer than all characteristic dimensions such as the size of the unit cell or the mean free path of the electrons. This is in general still fulﬁlled at ultraviolet frequencies3. Equation (1.10) reﬂects a certain arbitrariness in the separation of charges into bound and free sets, which is entirely due to convention. At low frequen- cies, ε is usually used for the description of the response of bound charges to a driving ﬁeld, leading to an electric polarization, while σ describes the contri- bution of free charges to the current ﬂow. At optical frequencies however, the distinction between bound and free charges is blurred. For example, for highly- doped semiconductors, the response of the bound valence electrons could be lumped into a static dielectric constant δε, and the response of the conduction electrons into σ , leading to a dielectric function ε(ω) = δε + iσ (ω) .Asimple ε0ω → → + ε0ω redeﬁnition δε 1andσ σ i δε will then result in the general form (1.10) [Ashcroft and Mermin, 1976]. In general, ε(ω) = ε1(ω)+iε2(ω) and σ(ω) = σ1(ω)+iσ2(ω) are complex- valued functions of angular frequency ω, linked via (1.10). At optical frequen- cies, ε can be experimentally determined for example via reﬂectivity studies and the determination of the complex√ refractive index n(ω)˜ = n(ω) + iκ(ω) of the medium, deﬁned as n˜ = ε. Explicitly, this yields

3However, spatial dispersion effects can lead to small corrections for surface plasmons polaritons in metallic nanostructures signiﬁcantly smaller than the electron mean free path, which can arise for example at the tip of metallic cones (see chapter 7). 10 Electromagnetics of Metals

2 2 ε1 = n − κ (1.11a) ε = 2nκ (1.11b) 2 ε 1 n2 = 1 + ε2 + ε2 (1.11c) 2 2 1 2 ε κ = 2 . (1.11d) 2n κ is called the extinction coefﬁcient and determines the optical absorption of electromagnetic waves propagating through the medium. It is linked to the absorption coefﬁcient α of Beer’s law (describing the exponential attenuation −αx of the intensity of a beam propagating through the medium via I(x)= I0e ) by the relation 2κ(ω)ω α(ω) = . (1.12) c Therefore, the imaginary part ε2 of the dielectric function determines the amount of absorption inside the medium. For |ε1| |ε2|, the real part n of the refractive index, quantifying the lowering of the phase velocity of the propagating waves due to polarization of the material, is mainly determined by ε1. Examination of (1.10) thus reveals that the real part of σ determines the amount of absorption, while the imaginary part contributes to ε1 and therefore to the amount of polarization. We close this section by examining traveling-wave solutions of Maxwell’s equations in the absence of external stimuli. Combining the curl equations (1.1c), (1.1d) leads to the wave equation

∂2D ∇×∇×E =−μ (1.13a) 0 ∂t2 ω2 K(K · E) − K2E =−ε(K,ω) E, (1.13b) c2 in the time and Fourier domains, respectively. c = √ 1 is the speed of light ε0μ0 in vacuum. Two cases need to be distinguished, depending on the polarization direction of the electric ﬁeld vector. For transverse waves, K · E = 0, yielding the generic dispersion relation

ω2 K2 = ε(K,ω) . (1.14) c2 For longitudinal waves, (1.13b) implies that

ε(K,ω)= 0, (1.15) The Dielectric Function of the Free Electron Gas 11 signifying that longitudinal collective oscillations can only occur at frequencies corresponding to zeros of ε(ω). We will return to this point in the discussion of volume plasmons in section 1.3.

1.2 The Dielectric Function of the Free Electron Gas Over a wide frequency range, the optical properties of metals can be ex- plained by a plasma model, where a gas of free electrons of number density n moves against a ﬁxed background of positive ion cores. For alkali metals, this range extends up to the ultraviolet, while for noble metals interband transi- tions occur at visible frequencies, limiting the validity of this approach. In the plasma model, details of the lattice potential and electron-electron interactions are not taken into account. Instead, one simply assumes that some aspects of the band structure are incorporated into the effective optical mass m of each electron. The electrons oscillate in response to the applied electromagnetic ﬁeld, and their motion is damped via collisions occurring with a characteristic collision frequency γ = 1/τ. τ is known as the relaxation time of the free electron gas, which is typically on the order of 10−14 s at room temperature, corresponding to γ = 100 THz. One can write a simple equation of motion for an electron of the plasma sea subjected to an external electric ﬁeld E:

mx¨ + mγ x˙ =−eE (1.16)

−iωt If we assume a harmonic time dependence E(t) = E0e of the driving ﬁeld, a particular solution of this equation describing the oscillation of the electron −iωt is x(t) = x0e . The complex amplitude x0 incorporates any phase shifts between driving ﬁeld and response via e x(t) = E(t). (1.17) m(ω2 + iγω) The displaced electrons contribute to the macroscopic polarization P =−nex, explicitly given by

ne2 P =− E. (1.18) m(ω2 + iγω) Inserting this expression for P into equation (1.2a) yields

ω2 D = ε (1 − p )E, (1.19) 0 ω2 + iγω

2 where ω2 = ne is the plasma frequency of the free electron gas. Therefore we p ε0m arrive at the desired result, the dielectric function of the free electron gas: 12 Electromagnetics of Metals

ω2 ε(ω) = 1 − p . (1.20) ω2 + iγω The real and imaginary components of this complex dielectric function ε(ω) = ε1(ω) + iε2(ω) are given by

ω2τ 2 ε (ω) = 1 − p (1.21a) 1 1 + ω2τ 2 ω2τ ε (ω) = p , (1.21b) 2 ω(1 + ω2τ 2) wherewehaveusedγ = 1/τ. It is insightful to study (1.20) for a variety of different frequency regimes with respect to the collision frequency γ . We will limit ourselves here to frequencies ω<ωp, where metals retain their metallic character. For large frequencies close to ωp, the product ωτ 1, leading to negligible damping. Here, ε(ω) is predominantly real, and

ω2 ε(ω) = 1 − p (1.22) ω2 can be taken as the dielectric function of the undamped free electron plasma. Note that the behavior of noble metals in this frequency region is completely altered by interband transitions, leading to an increase in ε2. The examples of gold and silver will be discussed below and in section 1.4. We consider next the regime of very low frequencies, where ω τ −1. Hence, ε2 ε1, and the real and the imaginary part of the complex refractive index are of comparable magnitude with ε τω2 n ≈ κ = 2 = p . (1.23) 2 2ω In this region, metals are mainly absorbing, with an absorption coefﬁcient of 1/2 2ω2τω α = p . (1.24) c2

By introducing the dc-conductivity σ0, this expression can be recast using = ne2τ = 2 σ0 m ωpτε0 to

α = 2σ0ωμ0. (1.25) The application of Beer’s law of absorption implies that for low frequencies the ﬁelds fall off inside the metal as e−z/δ,whereδ is the skin depth The Dielectric Function of the Free Electron Gas 13 2 c 2 δ = = = . (1.26) α κω σ0ωμ0 A more rigorous discussion of the low-frequency behavior based on the Boltzmann transport equation [Marder, 2000] shows that this description is indeed valid as long as the mean free path of the electrons l = vFτ δ,where vF is the Fermi velocity. At room temperature, for typical metals l ≈ 10 nm and δ ≈ 100 nm, thus justifying the free-electron model. At low temperatures however, the mean free path can increase by many orders of magnitude, lead- ing to changes in the penetration depth. This phenomenon is known as the anomalous skin effect. If we use σ instead of ε for the description of the dielectric response of metals, we recognize that in the absorbing regime it is predominantly real, and the free charge velocity responds in phase with the driving ﬁeld, as can be seen by integrating (1.17). At DC, relaxation effects of free charges are therefore conveniently described via the real DC-conductivity σ0, whereas the response of bound charges is put into a dielectric constant εB, as discussed above in the examination of the interlinked nature between ε and σ . At higher frequencies (1 ≤ ωτ ≤ ωpτ), the complex refractive index is predominantly imaginary (leading to a reﬂection coefﬁcient R ≈ 1 [Jackson, 1999]), and σ acquires more and more complex character, blurring the boundary between free and bound charges. In terms of the optical response, σ(ω)enters expressions only in the combination (1.10) [Ashcroft and Mermin, 1976], due to the arbitrariness of the division between free and bound sets discussed above. Whereas our description up to this point has assumed an ideal free-electron metal, we will now brieﬂy compare the model with an example of a real metal important in the ﬁeld of plasmonics (an extended discussion can be found in section 1.4). In the free-electron model, ε → 1atω ωp. For the noble metals (e.g. Au, Ag, Cu), an extension to this model is needed in the region ω>ωp (where the response is dominated by free s electrons), since the ﬁlled d band close to the Fermi surface causes a highly polarized environment. This residual polarization due to the positive background of the ion cores can be described by adding the term P∞ = ε0(ε∞ − 1)E to (1.2a), where P now represents solely the polarization (1.18) due to free electrons. This effect is therefore described by a dielectric constant ε∞ (usually 1 ≤ ε∞ ≤ 10), and we can write 2 ωp ε(ω) = ε∞ − . (1.27) ω2 + iγω The validity limits of the free-electron description (1.27) are illustrated for the case of gold in Fig. 1.1. It shows the real and imaginary components ε1 and ε2 for a dielectric function of this type, ﬁtted to the experimentally determined dielectric function of gold [Johnson and Christy, 1972]. Clearly, at visible 14 Electromagnetics of Metals

5 7 0 6

)] -5 5 ω )] ( ε ω

-10 ( 4 ε

Re[ region of -15 3 Im[ interband transitions -20 2 -25 1

001 2 3 4 5 6 1 2 3 4 5 6 Energy [eV] Energy [eV]

Figure 1.1. Dielectric function ε(ω) (1.27) of the free electron gas (solid line) ﬁtted to the literature values of the dielectric data for gold [Johnson and Christy, 1972] (dots). Interband transitions limit the validity of this model at visible and higher frequencies. frequencies the applicability of the free-electron model breaks down due to the occurrence of interband transitions, leading to an increase in ε2. This will be discussed in more detail in section 1.4. The components of the complex refractive index corresponding to the ﬁts presented in Fig. 1.1 are shown in Fig. 1.2. It is instructive to link the dielectric function of the free electron plasma (1.20) to the classical Drude model [Drude, 1900] for the AC conductivity σ(ω) of metals. This can be achieved by recognizing that equation (1.16) can be rewritten as p p˙ =− − eE, (1.28) τ where p = mx˙ is the momentum of an individual free electron. Via the same arguments presented above, we arrive at the following expression for the AC = nep conductivity σ m ,

2 10 1.75 8 1.5

) 1.25 6 ) ω ω

1 ( n( 0.75 κ 4 0.5 2 0.25

0.51 1.5 2 2.5 3 3.5 4 0.5 1 1.5 2 2.5 3 3.5 4 Energy [eV] Energy [eV]

Figure 1.2. Complex refractive index corresponding to the free-electron dielectric function in Fig. 1.1. The Dispersion of the Free Electron Gas and Volume Plasmons 15

σ σ(ω) = 0 . (1.29) 1 − iωτ By comparing equation (1.20) and (1.29), we get

iσ(ω) ε(ω) = 1 + , (1.30) ε0ω recovering the previous, general result of equation 1.10. The dielectric function of the free electron gas (1.20) is thus also known as the Drude model of the optical response of metals.

1.3 The Dispersion of the Free Electron Gas and Volume Plasmons We now turn to a description of the thus-far omitted transparency regime ω>ωp of the free electron gas model. Using equation (1.22) in (1.14), the dispersion relation of traveling waves evaluates to

2 = 2 + 2 2 ω ωp K c . (1.31) This relation is plotted for a generic free electron metal in Fig. 1.3. As can be seen, for ω<ωp the propagation of transverse electromagnetic waves is forbidden inside the metal plasma. For ω>ωp however, the plasma supports transverse waves propagating with a group velocity vg = dω/dK

2

plasma dispersion p ω / ω light line 1 Frequency

0 0 1 Wavevector Kc/ωp

Figure 1.3. The dispersion relation of the free electron gas. Electromagnetic wave propagation is only allowed for ω>ωp. 16 Electromagnetics of Metals

Figure 1.4. Longitudinal collective oscillations of the conduction electrons of a metal: Volume plasmons at the plasma frequency the electric ﬁeld is a pure depolarization ﬁeld, with E = −P . ε0 The physical signiﬁcance of the excitation at ωp can be understood by con- sidering the collective longitudinal oscillation of the conduction electron gas versus the ﬁxed positive background of the ion cores in a plasma slab. Schemat- ically indicated in Fig. 1.4, a collective displacement of the electron cloud by a distance u leads to a surface charge density σ =±neu at the slab boundaries. This establishes a homogeneous electric ﬁeld E = neu inside the slab. Thus, ε0 the displaced electrons experience a restoring force, and their movement can be described by the equation of motion nmu¨ =−neE. Inserting the expression for the electric ﬁeld, this leads to

n2e2u nmu¨ =− (1.32a) ε0

¨ + 2 = u ωpu 0. (1.32b)

The plasma frequency ωp can thus be recognized as the natural frequency of a free oscillation of the electron sea. Note that our derivation has assumed that all electrons move in phase, thus ωp corresponds to the oscillation frequency in the long-wavelength limit where K = 0. The quanta of these charge oscillations are called plasmons (or volume plasmons, to distinguish them from surface and localized plasmons, which will be discussed in the remainder of this text). Due to the longitudinal nature of the excitation, volume plasmons do not couple to transverse electromagnetic waves, and can only be excited by particle impact. Another consequence of this is that their decay occurs only via energy transfer to single electrons, a process known as Landau damping. Experimentally, the plasma frequency of metals typically is determined via electron loss spectroscopy experiments, where electrons are passed through thin metallic foils. For most metals, the plasma frequency is in the ultravio- let regime: ωp is on the order of 5 − 15 eV, depending on details of the band structure [Kittel, 1996]. As an aside, we want to note that such longitudinal os- Real Metals and Interband Transitions 17 cillations can also be excited in dielectrics, in which case the valence electrons oscillate collectively with respect to the ion cores. In addition to the in-phase oscillation at ωp, there exists a whole class of lon- gitudinal oscillations at higher frequencies with ﬁnite wavevectors, for which (1.15) is fulﬁlled. The derivation of the dispersion relation of volume plasmons is beyond the scope of this treatment and can be found in many textbooks on condensed matter physics [Marder, 2000, Kittel, 1996]. Up to quadratic order in K,

6E K2 ω2 = ω2 + F , (1.33) p 5m where EF is the Fermi energy. Practically, the dispersion can be measured us- ing inelastic scattering experiments such as electron energy loss spectroscopy (EELS).

1.4 Real Metals and Interband Transitions We have already on several occasions stated that the dielectric function (1.20) of the Drude model adequately describes the optical response of metals only for photon energies below the threshold of transitions between electronic bands. For some of the noble metals, interband effects already start to occur for energies in excess of 1 eV (corresponding to a wavelength λ ≈ 1 μm). As examples, Figs. 1.1 and 1.5 show the real and the imaginary parts ε1(ω), ε2(ω) of the dielectric function for gold and silver [Johnson and Christy, 1972] and Drude model ﬁts to the data. Clearly, this model is not adequate for describing either ε1 or ε2 at high frequencies, and in the case of gold, its validity breaks down already at the boundary between the near-infrared and the visible. We limit this comparison between the Drude model and the dielectric re- sponse of real metals to the cases of gold and silver, the most important metals for plasmonic studies in the visible and near-infrared. Above their respective

5 7 0 6

)] -5 5 )] ω ( ω ε -10 ( 4 ε

Re[ -15 3 Im[ -20 2 -25 1

00123456 123456 Energy [eV] Energy [eV]

Figure 1.5. The real and imaginary part of ε(ω) for silver determined by Johnson and Christy [Johnson and Christy, 1972] (dots) and a Drude model ﬁt to the data. 18 Electromagnetics of Metals band edge thresholds, photons are very efﬁcient in inducing interband tran- sitions, where electrons from the ﬁlled band below the Fermi surface are ex- cited to higher bands. Theoretically, these can be described using the same ap- proach used for direct band transitions in semiconductors [Ashcroft and Mer- min, 1976, Marder, 2000], and we will not embark on a more detailed discus- sion. The main consequence of these processes concerning surface plasmon polaritons is an increased damping and competition between the two excita- tions at visible frequencies. For practical purposes, a big advantage of the Drude model is that it can easily be incorporated into time-domain based numerical solvers for Maxwell’s equations, such as the ﬁnite-difference time-domain (FDTD) scheme [Kashiwa and Fukai, 1990], via the direct calculation of the induced currents using (1.16). Its inadequacy in describing the optical properties of gold and silver at visible frequencies can be overcome by replacing (1.16) by

¨ + ˙ + 2 =− mx mγ x mω0x eE. (1.34) Interband transitions are thus described using the classical picture of a bound electron with resonance frequency ω0, and (1.34) can then be used to calculate the resulting polarization. We note that a number of equations of this form might have to be solved (each resulting in a separate contribution to the total polarization) in order to model ε(ω) for noble metals accurately. Each of these Ai equations leads to a Lorentz-oscillator term of the form 2− 2− added to ωi ω iγi ω the free-electron result (1.20) [Vial et al., 2005].

1.5 The Energy of the Electromagnetic Field in Metals We ﬁnish this chapter by taking a brief look at the energy of the electro- magnetic ﬁeld inside metals, or more generally inside dispersive media. Since the amount of ﬁeld localization is often quantiﬁed in terms of the electromag- netic energy distribution, a careful consideration of the effects of dispersion is necessary. For a linear medium with no dispersion or losses (i.e. (1.5) holds), the total energy density of the electromagnetic ﬁeld can be written as [Jackson, 1999] 1 u = (E · D + B · H). (1.35) 2 This expression enters together with the Poynting vector of energy ﬂow S = E × H into the conservation law ∂u +∇·S =−J · E, (1.36) ∂t relating changes in electromagnetic energy density to energy ﬂow and absorp- tion inside the material. The Energy of the Electromagnetic Field in Metals 19

In the following, we will concentrate on the contribution uE of the electric ﬁeld E to the total electromagnetic energy density. In metals, ε is complex and frequency-dependent due to dispersion, and (1.35) does not apply. For a ﬁeld consisting of monochromatic components, Landau and Lifshitz have shown that the conservation law (1.36) can be held up if uE is replaced by an effective electric energy density ueff,deﬁnedas

1 d(ωε) u = Re E(r,t)· E(r,t) , (1.37) eff 2 dω ω0 where E(r,t)· E(r,t) signiﬁes ﬁeld-averaging over one optical cycle, and ω0 is the frequency of interest. This expression is valid if E is only apprecia- ble in a narrow frequency range around ω0, and the ﬁelds are slowly-varying compared to a timescale 1/ω0. Furthermore, it is assumed that |ε2| |ε1|, so that absorption is small. We note that additional care must be taken with the correct calculation of absorption on the right side of (1.36), where J · E should be replaced by ω0Im [ε(ω0)] E(r,t)· E(r,t) if the dielectric response of the metal is completely described via ε(ω) [Jackson, 1999], in line with the discussion surrounding (1.10). The requirement of low absorption limits (1.37) to visible and near-infrared frequencies, but not to lower frequencies or the regime of interband effects where |ε2| > |ε1|. However, the electric ﬁeld energy can also be determined by taking the electric polarization explicitly into account, in the form described by (1.16) [Loudon, 1970, Ruppin, 2002]. The obtained expression for the electric ﬁeld energy of a material described by a free-electron-type dielectric function ε = ε1 + iε2 of the form (1.20) is

ε 2ωε u = 0 ε + 2 |E|2 , (1.38) eff 4 1 γ where an additional factor 1/2 is included due to an implicit assumption of harmonic time dependence of the oscillating ﬁelds. For negligible ε2,itcanbe shown that (1.38) reduces as expected to (1.37) for time-harmonic ﬁelds. We will use (1.38) in chapter 2 when discussing the amount of energy localization in ﬁelds localized at metallic surfaces. Chapter 2

SURFACE PLASMON POLARITONS AT METAL / INSULATOR INTERFACES

Surface plasmon polaritons are electromagnetic excitations propagating at the interface between a dielectric and a conductor, evanescently conﬁned in the perpendicular direction. These electromagnetic surface waves arise via the coupling of the electromagnetic ﬁelds to oscillations of the conductor’s electron plasma. Taking the wave equation as a starting point, this chapter describes the fundamentals of surface plasmon polaritons both at single, ﬂat interfaces and in metal/dielectric multilayer structures. The surface excitations are characterized in terms of their dispersion and spatial proﬁle, together with a detailed discussion of the quantiﬁcation of ﬁeld conﬁnement. Applications of surface plasmon polaritons in waveguiding will be deferred to chapter 7.

2.1 The Wave Equation In order to investigate the physical properties of surface plasmon polaritons (SPPs), we have to apply Maxwell’s equations (1.1) to the ﬂat interface be- tween a conductor and a dielectric. To present this discussion most clearly, it is advantageous to cast the equations ﬁrst in a general form applicable to the guiding of electromagnetic waves, the wave equation. As we have seen in chapter 1, in the absence of external charge and current densities, the curl equations (1.1c, 1.1d) can be combined to yield

∂2D ∇×∇×E =−μ . (2.1) 0 ∂t2

Using the identities ∇×∇×E ≡∇(∇·E) −∇2E as well as ∇·(εE) ≡ E ·∇ε + ε∇·E, and remembering that due to the absence of external stimuli ∇·D = 0, (2.1) can be rewritten as 22 Surface Plasmon Polaritons at Metal / Insulator Interfaces

1 ∂2E ∇ − E ·∇ε −∇2E =−μ ε ε . (2.2) ε 0 0 ∂t2

For negligible variation of the dielectric proﬁle ε = ε(r) over distances on the order of one optical wavelength, (2.2) simpliﬁes to the central equation of electromagnetic wave theory,

ε ∂2E ∇2E − = 0. (2.3) c2 ∂t2

Practically, this equation has to be solved separately in regions of constant ε, and the obtained solutions have to been matched using appropriate boundary conditions. To cast (2.3) in a form suitable for the description of conﬁned propagating waves, we proceed in two steps. First, we assume in all generality a harmonic time dependence E(r,t)= E(r)e−iωt of the electric ﬁeld. Inserted into (2.3), this yields

∇2 + 2 = E k0εE 0, (2.4)

= ω where k0 c is the wave vector of the propagating wave in vacuum. Equation (2.4) is known as the Helmholtz equation. Next, we have to deﬁne the propagation geometry. We assume for sim- plicity a one-dimensional problem, i.e. ε depends only on one spatial coor- dinate. Speciﬁcally, the waves propagate along the x-direction of a cartesian coordinate system, and show no spatial variation in the perpendicular, in-plane y-direction (see Fig. 2.1); therefore ε = ε(z). Applied to electromagnetic surface problems, the plane z = 0 coincides with the interface sustaining the

z x (direction of propagation) y

Figure 2.1. Deﬁnition of a planar waveguide geometry. The waves propagate along the x- direction in a cartesian coordinate system. The Wave Equation 23 propagating waves,which can now be described as E(x,y,z)= E(z)eiβx .The complex parameter β = kx is called the propagation constant of the traveling waves and corresponds to the component of the wave vector in the direction of propagation. Inserting this expression into (2.4) yields the desired form of the wave equation

∂2E(z) + k2ε − β2 E = 0. (2.5) ∂z2 0 Naturally, a similar equation exists for the magnetic ﬁeld H. Equation (2.5) is the starting point for the general analysis of guided elec- tromagnetic modes in waveguides, and an extended discussion of its properties and applications can be found in [Yariv, 1997] and similar treatments of pho- tonics and optoelectronics. In order to use the wave equation for determining the spatial ﬁeld proﬁle and dispersion of propagating waves, we now need to ﬁnd explicit expressions for the different ﬁeld components of E and H.This can be achieved in a straightforward way using the curl equations (1.1c, 1.1d). ∂ =− For harmonic time dependence ∂t iω , we arrive at the following set of coupled equations

∂E ∂E z − y = iωμ H (2.6a) ∂y ∂z 0 x

∂E ∂E x − z = iωμ H (2.6b) ∂z ∂x 0 y

∂E ∂E y − x = iωμ H (2.6c) ∂x ∂y 0 z

∂H ∂H z − y =−iωε εE (2.6d) ∂y ∂z 0 x

∂H ∂H x − z =−iωε εE (2.6e) ∂z ∂x 0 y

∂H ∂H y − x =−iωε εE . (2.6f) ∂x ∂y 0 z ∂ = For propagation along the x-direction ∂x iβ and homogeneity in the y- ∂ = direction ∂y 0 , this system of equation simpliﬁes to 24 Surface Plasmon Polaritons at Metal / Insulator Interfaces

∂E y =−iωμ H (2.7a) ∂z 0 x ∂E x − iβE = iωμ H (2.7b) ∂z z 0 y iβEy = iωμ0Hz (2.7c) ∂H y = iωε εE (2.7d) ∂z 0 x ∂H x − iβH =−iωε εE (2.7e) ∂z z 0 y iβHy =−iωε0εEz. (2.7f) It can easily be shown that this system allows two sets of self-consistent solutions with different polarization properties of the propagating waves. The ﬁrst set are the transverse magnetic (TM or p) modes, where only the ﬁeld components Ex, Ez and Hy are nonzero, and the second set the transverse electric (TE or s) modes, with only Hx, Hz and Ey being nonzero. For TM modes, the system of governing equations (2.7) reduces to

1 ∂Hy Ex =−i (2.8a) ωε0ε ∂z β Ez =− Hy, (2.8b) ωε0ε and the wave equation for TM modes is ∂2H y + k2ε − β2 H = 0. (2.8c) ∂z2 0 y For TE modes the analogous set is

1 ∂Ey Hx = i (2.9a) ωμ0 ∂z β Hz = Ey, (2.9b) ωμ0 with the TE wave equation ∂2E y + k2ε − β2 E = 0. (2.9c) ∂z2 0 y With these equations at our disposal, we are now in a position to embark on the description of surface plasmon polaritons. Surface Plasmon Polaritons at a Single Interface 25 2.2 Surface Plasmon Polaritons at a Single Interface The most simple geometry sustaining SPPs is that of a single, ﬂat interface (Fig. 2.2) between a dielectric, non-absorbing half space (z>0) with positive real dielectric constant ε2 and an adjacent conducting half space (z<0) de- scribed via a dielectric function ε1(ω). The requirement of metallic character implies that Re [ε1] < 0. As shown in chapter 1, for metals this condition is fulﬁlled at frequencies below the bulk plasmon frequency ωp. We want to look for propagating wave solutions conﬁned to the interface, i.e. with evanescent decay in the perpendicular z-direction. Let us ﬁrst look at TM solutions. Using the equation set (2.8) in both half spaces yields

iβx −k2z Hy(z) = A2e e (2.10a) 1 iβx −k2z Ex(z) = iA2 k2e e (2.10b) ωε0ε2 β iβx −k2z Ez(z) =−A1 e e (2.10c) ωε0ε2 for z>0and

iβx k1z Hy(z) = A1e e (2.11a) 1 iβx k1z Ex(z) =−iA1 k1e e (2.11b) ωε0ε1 β iβx k1z Ez(z) =−A1 e e (2.11c) ωε0ε1 for z<0. ki ≡ kz,i(i = 1, 2) is the component of the wave vector perpen- dicular to the interface in the two media. Its reciprocal value, zˆ = 1/ |kz|, deﬁnes the evanescent decay length of the ﬁelds perpendicular to the interface,

z

x Dielectric

Metal

Figure 2.2. Geometry for SPP propagation at a single interface between a metal and a dielec- tric. 26 Surface Plasmon Polaritons at Metal / Insulator Interfaces which quantiﬁes the conﬁnement of the wave. Continuity of Hy and εiEz at the interface requires that A1 = A2 and k ε 2 =− 2 . (2.12) k1 ε1 Note that with our convention of the signs in the exponents in (2.10,2.11), conﬁnement to the surface demands Re [ε1] < 0ifε2 > 0 - the surface waves exist only at interfaces between materials with opposite signs of the real part of their dielectric permittivities, i.e. between a conductor and an insulator. The expression for Hy further has to fulﬁll the wave equation (2.8c), yielding

2 = 2 − 2 k1 β k0ε1 (2.13a) 2 = 2 − 2 k2 β k0ε2. (2.13b) Combining this and (2.12) we arrive at the central result of this section, the dispersion relation of SPPs propagating at the interface between the two half spaces ε1ε2 β = k0 . (2.14) ε1 + ε2

This expression is valid for both real and complex ε1, i.e. for conductors with- out and with attenuation. Before discussing the properties of the dispersion relation (2.14) in more detail, we now brieﬂy analyze the possibility of TE surface modes. Using (2.9), the respective expressions for the ﬁeld components are

iβx −k2z Ey(z) = A2e e (2.15a) 1 iβx −k2z Hx(z) =−iA2 k2e e (2.15b) ωμ0 β iβx −k2z Hz(z) = A2 e e (2.15c) ωμ0 for z>0and

iβx k1z Ey(z) = A1e e (2.16a) 1 iβx k1z Hx(z) = iA1 k1e e (2.16b) ωμ0 β iβx k1z Hz(z) = A1 e e (2.16c) ωμ0 Surface Plasmon Polaritons at a Single Interface 27

air silica 1 p ω / 0.8 ω

ω sp,air 0.6 ωsp,silica 0.4 Frequency Frequency 0.2

0 0 1

Wave vector βc/ωp

Figure 2.3. Dispersion relation of SPPs at the interface between a Drude metal with negligible collision frequency and air (gray curves) and silica (black curves). for z<0. Continuity of Ey and Hx at the interface leads to the condition

A1 (k1 + k2) = 0. (2.17)

Since conﬁnement to the surface requires Re [k1] > 0andRe[k2] > 0, this condition is only fulﬁlled if A1 = 0, so that also A2 = A1 = 0. Thus, no surface modes exist for TE polarization. Surface plasmon polaritons only exist for TM polarization. We now want to examine the properties of SPPs by taking a closer look at their dispersion relation. Fig. 2.3 shows plots of (2.14) for a metal with negli- gible damping described by the real Drude dielectric function (1.22) for an air (ε2 = 1) and a fused silica (ε2 = 2.25) interface. In this plot, the frequency ω is normalized to the plasma frequency ωp, and both the real (continuous curves) and the imaginary part (broken curves) of the wave vector β are shown. Due to their bound nature, the SPP excitations correspond to the part of the dis- persion curves lying to the right of the respective light lines of air and silica. Thus, special phase-matching techniques such as grating or prism coupling are required for their excitation via three-dimensional beams, which will be dis- cussed in chapter 3. Radiation into the metal occurs in the transparency regime ω>ωp as mentioned in chapter 1. Between the regime of the bound and radiative modes, a frequency gap region with purely imaginary β prohibiting propagation exists. For small wave vectors corresponding to low (mid-infrared or lower) fre- quencies, the SPP propagation constant is close to k0 at the light line, and the 28 Surface Plasmon Polaritons at Metal / Insulator Interfaces waves extend over many wavelengths into the dielectric space. In this regime, SPPs therefore acquire the nature of a grazing-incidence light ﬁeld, and are also known as Sommerfeld-Zenneck waves [Goubau, 1950]. In the opposite regime of large wave vectors, the frequency of the SPPs approaches the characteristic surface plasmon frequency

ωp ωsp = √ , (2.18) 1 + ε2 as can be shown by inserting the free-electron dielectric function (1.20) into (2.14). In the limit of negligible damping of the conduction electron oscillation (implying Im [ε1(ω)] = 0), the wave vector β goes to inﬁnity as the frequency approaches ωsp, and the group velocity vg → 0. The mode thus acquires electrostatic character, and is known as the surface plasmon. It can indeed be obtained via a straightforward solution of the Laplace equation ∇2φ = 0for the single interface geometry of Fig. 2.2, where φ is the electric potential. A solution that is wavelike in the x-direction and exponentially decaying in the z-direction is given by

iβx −k2z φ(z) = A2e e (2.19) for z>0and

iβx k1z φ(z) = A1e e (2.20) 2 for z< 0. ∇ φ = 0 requires that k1 = k2 = β: the exponential decay lengths zˆ = 1/kz into the dielectric and into the metal are equal. Continuity of φ and ε∂φ/∂z ensure continuity of the tangential ﬁeld components and the normal components of the dielectric displacement and require that A1 = A2 and additionally

ε1(ω) + ε2 = 0. (2.21) For a metal described by a dielectric function of the form (1.22), this condi- tion is fulﬁlled at ωsp. Comparison of (2.21) and (2.14) show that the surface plasmon is indeed the limiting form of a SPP as β →∞. The above discussions of Fig. 2.3 have assumed an ideal conductor with Im [ε1] = 0. Excitations of the conduction electrons of real metals however suffer both from free-electron and interband damping. Therefore, ε1(ω) is complex, and with it also the SPP propagation constant β. The traveling SPPs are damped with an energy attenuation length (also called propagation length) L = (2Im β )−1, typically between 10 and 100 μm in the visible regime, depending upon the metal/dielectric conﬁguration in question. Fig. 2.4 shows as an example the dispersion relation of SPPs propagating at a silver/air and silver/silica interface, with the dielectric function ε1(ω) of silver Surface Plasmon Polaritons at a Single Interface 29

10 air silica 8 Hz] 15

[10 6 ω 4

2 Frequency Frequency

0 024 68 Wave vector Re{β }[107 m-1]

Figure 2.4. Dispersion relation of SPPs at a silver/air (gray curve) and silver/silica (black curve) interface. Due to the damping, the wave vector of the bound SPPs approaches a ﬁnite limit at the surface plasmon frequency. taken from the data obtained by Johnson and Christy [Johnson and Christy, 1972]. Compared with the dispersion relation of completely undamped SPPs depicted in Fig. 2.3, it can be seen that the bound SPPs approach now a maxi- mum, ﬁnite wave vector at the the surface plasmon frequency ωsp of the system. This limitation puts a lower bound both on the wavelength λsp = 2π/Re β of the surface plasmon and also on the amount of mode conﬁnement perpen- −| || | dicular to the interface, since the SPP ﬁelds in the dielectric fall off as e kz z = 2 − ω 2 with kz β ε2 c . Also, the quasibound, leaky part of the dispersion relation between ωsp and ωp is now allowed, in contrast to the case of an ideal conductor, where Re β = 0 in this regime (Fig. 2.3). We ﬁnish this section by providing an example of the propagation length L and the energy conﬁnement (quantiﬁed by zˆ) in the dielectric. As is evident from the dispersion relation, both show a strong dependence on frequency. SPPs at frequencies close to ωsp exhibit large ﬁeld conﬁnement to the inter- face and a subsequent small propagation distance due to increased damping. Using the theoretical treatment outlined above, we see that SPPs at a silver/air interface at λ0 = 450 nm for example have L ≈ 16 μmandzˆ ≈ 180 nm. At λ0 ≈ 1.5 μmhowever,L ≈ 1080 μmandzˆ ≈ 2.6 μm. The better the conﬁnement, the lower the propagation length. This characteristic trade-off between localization and loss is typical for plasmonics. We note that ﬁeld- conﬁnement below the diffraction limit of half the wavelength in the dielectric can be achieved close to ωsp. In the metal itself, the ﬁelds fall off over distances 30 Surface Plasmon Polaritons at Metal / Insulator Interfaces on the order of 20 nm over a wide frequency range spanning from the visible to the infrared.

2.3 Multilayer Systems We now turn our attention to SPPs in multilayers consisting of alternating conducting and dielectric thin ﬁlms. In such a system, each single interface can sustain bound SPPs. When the separation between adjacent interfaces is comparable to or smaller than the decay length zˆ of the interface mode, in- teractions between SPPs give rise to coupled modes. In order to elucidate the general properties of coupled SPPs, we will focus on two speciﬁc three- layer systems of the geometry depicted in Fig. 2.5: Firstly, a thin metallic layer (I) sandwiched between two (inﬁnitely) thick dielectric claddings (II, III), an insulator/metal/insulator (IMI) heterostructure, and secondly a thin di- electric core layer (I) sandwiched between two metallic claddings (II, III), a metal/insulator/metal (MIM) heterostructure. Since we are here only interested in the lowest-order bound modes, we start with a general description of TM modes that are non-oscillatory in the z-direction normal to the interfaces using (2.8). For z>a, the ﬁeld compo- nents are

iβx −k3z Hy = Ae e (2.22a) 1 iβx −k3z Ex = iA k3e e (2.22b) ωε0ε3 β iβx −k3z Ez =−A e e , (2.22c) ωε0ε3 while for z<−a we get

z

III a I -a x II

Figure 2.5. Geometry of a three-layer system consisting of a thin layer I sandwiched between two inﬁnite half spaces II and III. Multilayer Systems 31

iβx k2z Hy = Be e (2.23a) 1 iβx k2z Ex =−iB k2e e (2.23b) ωε0ε2 β iβx k2z Ez =−B e e . (2.23c) ωε0ε2 Thus, we demand that the ﬁelds decay exponentially in the claddings (II) and (III). Note that for simplicity as before we denote the component of the wave vector perpendicular to the interfaces simply as ki ≡ kz,i. Inthecoreregion−a

iβx k1z iβx −k1z Hy = Ce e + De e (2.24a) 1 1 iβx k1z iβx −k1z Ex =−iC k1e e + iD k1e e (2.24b) ωε0ε1 ωε0ε1 β β iβx k1z iβx −k1z Ez = C e e + D e e . (2.24c) ωε0ε1 ωε0ε1

The requirement of continutity of Hy and Ex leads to

− − Ae k3a = Cek1a + De k1a (2.25a) A C D −k3a k1a −k1a k3e =− k1e + k1e (2.25b) ε3 ε1 ε1 at z = a and

− − Be k2a = Ce k1a + Dek1a (2.26a) B C D −k2a −k1a k1a − k2e =− k1e + k1e (2.26b) ε2 ε1 ε1 at z =−a, a linear system of four coupled equations. Hy further has to fulﬁll the wave equation (2.8c) in the three distinct regions, via

2 = 2 − 2 ki β k0εi (2.27) for i = 1, 2, 3. Solving this system of linear equations results in an implicit expression for the dispersion relation linking β and ω via

− k1/ε1 + k2/ε2 k1/ε1 + k3/ε3 e 4k1a = . (2.28) k1/ε1 − k2/ε2 k1/ε1 − k3/ε3 32 Surface Plasmon Polaritons at Metal / Insulator Interfaces

We note that for inﬁnite thickness (a →∞), (2.28) reduces to (2.12), the equation of two uncoupled SPP at the respective interfaces. We will from this point onwards consider the interesting special case where the sub- and the superstrates (II) and (III) are equal in terms of their dielectric response, i.e. ε2 = ε3 and thus k2 = k3. In this case, the dispersion relation (2.28) can be split into a pair of equations, namely

k2ε1 tanh k1a =− (2.29a) k1ε2 k1ε2 tanh k1a =− . (2.29b) k2ε1 It can be shown that equation (2.29a) describes modes of odd vector parity (Ex(z) is odd, Hy(z) and Ez(z) are even functions), while (2.29b) describes modes of even vector parity (Ex(z) is even function, Hy(z) and Ez(z) are odd). The dispersion relations (2.29a, 2.29b) can now be applied to IMI and MIM structures to investigate the properties of the coupled SPP modes in these two systems. We ﬁrst start with the IMI geometry - a thin metallic ﬁlm of thick- ness 2a sandwiched between two insulating layers. In this case ε1 = ε1(ω) represents the dielectric function of the metal, and ε2 the positive, real dielec- tric constant of the insulating sub- and superstrates. As an example, Fig. 2.6 shows the dispersion relations of the odd and even modes (2.29a, 2.29b) for an air/silver/air geometry for two different thicknesses of the silver thin ﬁlm. For

8

odd modes ω+

Hz] 6

15 even modes ω− [10

ω 4

2 Frequency 0 0 2468 Wave vector β [107 m-1]

Figure 2.6. Dispersion relation of the coupled odd and even modes for an air/silver/air mul- tilayer with a metal core of thickness 100 nm (dashed gray curves) and 50 nm (dashed black curves). Also shown is the dispersion of a single silver/air interface (gray curve). Silver is modeled as a Drude metal with negligible damping. Multilayer Systems 33 simplicity, here the dielectric function of silver is approximated via a Drude model with negligible damping (ε(ω) real and of the form (1.22)), so that Im β = 0. As can be seen, the odd modes have frequencies ω+ higher than the respec- tive frequencies for a single interface SPP, and the even modes lower frequen- cies ω−. For large wave vectors β (which are only achievable if Im [ε(ω)] = 0), the limiting frequencies are −2βa ωp 2ε2e ω+ = √ 1 + (2.30a) 1 + ε 1 + ε 2 2 −2βa ωp 2ε2e ω− = √ − . 1 + (2.30b) 1 + ε2 1 ε2 Odd modes have the interesting property that upon decreasing metal ﬁlm thickness, the conﬁnement of the coupled SPP to the metal ﬁlm decreases as the mode evolves into a plane wave supported by the homogeneous dielectric environment. For real, absorptive metals described via a complex ε(ω),this implies a drastically increased SPP propagation length [Sarid, 1981]. These long-ranging SPPs will be further discussed in chapter 7. The even modes exhibit the opposite behavior - their conﬁnement to the metal increases with decreasing metal ﬁlm thickness, resulting in a reduction in propagation length. Moving on to MIM geometries, we now set ε2 = ε2(ω) as the dielectric function of the metal and ε1 as the dielectric constant of the insulating core in equations (2.29a, 2.29b). From an energy conﬁnement point of view, the most interesting mode is the fundamental odd mode of the system, which does not exhibit a cut-off for vanishing core layer thickness [Prade et al., 1991]. Fig. 2.7 shows the dispersion relation of this mode for a silver/air/silver het- erostructure. This time, the dielectric function ε(ω) was taken as a complex ﬁt to the dielectric data of silver obtained by Johnson and Christy [Johnson and Christy, 1972]. Thus β does not go to inﬁnity as the surface plasmon frequency is approached, but folds back and eventually crosses the light line, as for SPPs propagating at single interfaces. It is apparent that large propagation constants β can be achieved even for excitation well below ωsp, provided that the width of the dielectric core is cho- sen sufﬁciently small. The ability to access such large wave vectors and thus small penetration lengths zˆ into the metallic layers by adjusting the geometry indicates that localization effects that for a single interface can only be sus- tained at excitations near ωsp, can for such MIM structures also be attained for excitation out in the the infrared. An analysis of various other MIM structures, for example concentric shells, has given similar results [Takahara et al., 1997]. Geometries amendable to easy fabrication such as triangular metal V-grooves 34 Surface Plasmon Polaritons at Metal / Insulator Interfaces

6 Hz] 15 4

[10 2a ω Ag air Ag

2 x |Ez| Frequency Frequency z 0 024 68 Wave vector Re{β}[107 m-1]

Figure 2.7. Dispersion relation of the fundamental coupled SPP modes of a silver/air/silver multilayer geometry for an air core of size 100 nm (broken gray curve), 50 nm (broken black curve), and 25 nm (continuous black curve). Also shown is the dispersion of a SPP at a single silver/air interface (gray curve) and the air light line (gray line). on a ﬂat metal surface have already shown great promise for applications in waveguiding, which will be presented in chapter 7. We have limited our discussion of coupled SPPs in three-layer structures to the fundamental bound modes of the system, with a view on applications in waveguiding and conﬁnement of electromagnetic energy. It is important to note that the family of modes supported by this geometry is much richer than described in this treatment. For example, for IMI structures, we have omitted a discussion of leaky modes, and MIM layers can also exhibit oscillatory modes for sufﬁcient thickness of the dielectric core. Additionally, the coupling be- tween SPPs at the two core/cladding interfaces changes signiﬁcantly when the dielectric constants of the sub- and superstrates are different, so that ε2 = ε3, prohibiting phase-matching between the modes located at the two interfaces. A detailed treatment of these cases can be found in [Economou, 1969, Burke and Stegeman, 1986, Prade et al., 1991].

2.4 Energy Conﬁnement and the Effective Mode Length In chapter 5 we will see that using localized surface plasmons in metal nanoparticles, electromagnetic energy can be conﬁned or squeezed√ into vol- 3 umes smaller than the diffraction limit (λ0/2n) ,wheren = ε is the re- fractive index of the surrounding medium. This high conﬁnement leads to a concomitant ﬁeld enhancement and is of prime importance in plasmonics, en- abling a great variety of applications in optical sensing, as will be discussed in chapter 9. In the essentially one-dimensional cases of single interfaces and Energy Conﬁnement and the Effective Mode Length 35

(a) (b) 100 2 10

0 1

/k 1 β 0.1

0.1 % energy in metal 0.01 10 20 80 10-4 10-3 10-2 10-1 1 10 Gap size 2a [nm] normalized gap size

(c) 10

eff 1 _

10-1

10-2

10-3 Mode Length, L Mode Length, 10-4 10-4 10-3 10-2 10-1 1 10 normalized gap size

Figure 2.8. Energy conﬁnement in a gold/air/gold MIM structure. (a) Real (solid curve) and imaginary (dashed curve) part of the normalized propagation constant β versus gap size at λ0 = 850nm. (b) Fraction of electric ﬁeld energy residing inside the metallic half spaces as a function of normalized gap size for excitation at λ0 = 600 nm (thick curve), 850nm (black curve), 1.5 μm (gray curve), 10 μm (broken black curve), and 100 μm (broken gray curve). (c) Effective mode length Leff normalized to free-space wavelength λ0 as a function of gap size. Adapted from [Maier, 2006b]. multilayer structures presented above that support propagating SPPs, energy localization below the diffraction limit perpendicular to the interface(s) is also possible. We have already hinted at this phenomenon when stating that the ﬁeld decay length zˆ in the dielectric layers can be signiﬁcantly smaller than λ0/n. However, care must be taken when quantifying energy conﬁnement, since a sub-wavelength ﬁeld decay length zˆ on the dielectric side of the interface implies that a signiﬁcant amount of the total electric ﬁeld energy of the SPP mode resides inside the metal. This energy must be taken into account using (1.38) when calculating the spatial distribution of the electric energy density, since for the quantiﬁcation of the strength of interactions between light and matter (e.g. a molecule placed into the ﬁeld), the ﬁeld strength per unit energy (i.e., single photon) is of importance. Taking a gold/air/gold MIM heterostructure as an example, Fig. 2.8(a) shows the evolution of both the real and imaginary parts of the propagation constant β of the fundamental SPP mode with varying gap size for excitation at a free space wavelength of λ0 = 850 nm, calculated using Drude ﬁts to the dielectric 36 Surface Plasmon Polaritons at Metal / Insulator Interfaces function of gold [Johnson and Christy, 1972, Ordal et al., 1983]. Both parts increase with decreasing gap size, since the mode is becoming more electron- plasma in character, suggesting that the electromagnetic energy is residing in- creasingly in the metal half-spaces. A plot of the fractional amount of the electric ﬁeld energy inside the metal regions is shown in Fig. 2.8(b) for exci- tation at wavelengths λ0 = 600 nm, 850 nm, 1.5 μm, 10 μm, and 100 μm (= 3THz). For a gap of 20 nm for example, at λ0 = 850 nm this fraction al- ready reaches 40%. Note that the gap size is normalized to the respective free space wavelength. It is apparent that along with the increased localization of the ﬁeld to the gold/air interface, either via small gap sizes or excitation closer to ωsp, comes a shift of the energy into the metal regions. In order to get a better handle on the consequences of increasing fractions of the total energy of the mode entering the metallic cladding upon decreasing size of the dielectric gap, we can deﬁne in analogy to the effective mode volume Veff used to quantify the strength of light-matter interactions in cavity quantum electrodynamics [Andreani et al., 1999] an effective mode length Leff, with

Leff(z0)ueff(z0) = ueff(z)dz. (2.31) ueff(z0) represents the electric ﬁeld energy density at a position z0 of interest within the air core (e.g. the location of an emitter). In this one-dimensional picture, the effective mode length is therefore given as the ratio of the total energy of the SPP mode divided by the energy density (energy per unit length) at the position of interest, which is often taken as the position of highest ﬁeld. In a quantized picture for normalized total energy, the inverse of the effective mode length thus quantiﬁes the ﬁeld strength per single SPP excitation. More details can be found in [Maier, 2006b]. A determination of the effective mode length of MIM structures allows an examination how the electric ﬁeld strength per SPP excitation in the air gap ¯ scales as a function of the gap size. Fig. 2.8(c) shows the variation of Leff (normalized to the free-space wavelength λ0) with normalized gap size. z0 is taken to be at the air side of the air/gold boundary, where the electric ﬁeld strength is maximum. The mode lengths drop well below λ0/2, demonstrating that plasmonic metal structures can indeed sustain effective as well as physical mode lengths below the diffraction limit of light. The trend in Leff with gap size tends to scale with the physical extent of the air gap. For large normalized gap sizes and low frequencies, this is due to the delocalized nature of the surface plasmon, leading to smaller mode lengths for excitation closer to the surface plasmon frequency ωsp for the same normalized gap size. As the gap size is reduced to a point where the dispersion curve of the SPP mode turns over (see Fig. 2.7) and energy begins to enter the metallic half spaces, the continued reduction in mode length is due to an increase in ﬁeld Energy Conﬁnement and the Effective Mode Length 37 localization to the metal-air interface. In this regime, excitations with lower frequencies show smaller mode lengths for the same normalized gap size than excitations closer to the plasmon resonance, due to the fact that more energy resides inside the metal for the latter. We note that for very small gaps with 2a<2 nm, the effects of local ﬁelds due to unscreened surface electrons become important [Larkin et al., 2004], leading to a further decrease in Leff. This cannot be captured using the dielectric function approach. To summarize, we see that despite the penetration of a signiﬁcant amount of energy of a SPP mode into the conducting medium (for excitation near ωsp or in small gap structures), the associated large propagation constants β ensure that the effective extent of the mode perpendicular to the interface(s) drops well below the diffraction limit.